- About this Journal ·
- Abstracting and Indexing ·
- Advance Access ·
- Aims and Scope ·
- Annual Issues ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

Journal of Nanomaterials

Volume 2012 (2012), Article ID 278364, 6 pages

http://dx.doi.org/10.1155/2012/278364

## Femtosecond Laser-Induced Formation of Wurtzite Phase ZnSe Nanoparticles in Air

^{1}Department of Electrophysics, National Chiao Tung University, Hsinchu 30010, Taiwan^{2}Graduate Institute of Electro-optical Engineering, Tatung University, Taipei 104, Taiwan^{3}Advanced Ultrafast Laser Research Center and Department of Engineering Science, Faculty of Informatics and Engineering, The University of Electro-Communications, 1-5-1 Chofugaoka, Chofu, Tokyo 182-8585, Japan

Received 27 March 2012; Revised 21 June 2012; Accepted 9 July 2012

Academic Editor: Marinella Striccoli

Copyright © 2012 Hsuan I Wang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

We demonstrate an effective method to prepare wurtzite phase ZnSe nanoparticles from zincblende ZnSe single crystal using femtosecond pulse laser ablation. The fabricated ZnSe nanoparticles are in spherical shape and uncontaminated while synthesized under ambient environment. By controlling the laser fluences, the average size of ZnSe nanoparticles can be varied from *~*16 nm to *~*22 nm in diameter. In Raman spectra, the surface phonon mode becomes dominant in the smaller average particle size with uniform size distribution. The interesting phase transition from the zinc blende structure of ZnSe single crystal to wurtzite structure of ZnSe nanoparticles may have been induced by the ultrahigh ablation pressure at the local area due to the sudden injection of high energy leading to solid-solid transition.

The nanometer sized materials have provided an opportunity to study the relation between material properties and size. Due to the uniquely dimension-dependent properties, the nanosized material has the potential for various applications such as nanoelectronics, nanosensors, nanooptronics, and chemical catalyst [1–3]. The nanostructures of zinc selenide (ZnSe), in particular, have attracted considerable attention. ZnSe is an important II–VI semiconductor due to its promising optoelectrical and electrical properties of direct wide band gap 2.68 eV at 300 K. The ZnSe nanoparticles can be obtained through chemical reduction [4], vapor synthesis [5], or laser ablation method [6]. Generally, crystalline ZnSe exhibits two structural phases, that is, zinc blende and wurtzite [7]. However, the studies on wurtzite phase ZnSe nanoparticles are few [8–10] owing to that the wurtzite structure is thermodynamically unstable in ambient environments and requires the critical growth conditions. Recently, the femtosecond (fs) laser ablation has been extensively used for material processing [11–15]. Because of the unique features, in fs time-scale pulse duration and high power density (~GW/cm^{2}), the high quality nanosized materials can be obtained without thermal effects. For instance, nanospike [12], nanowire [14], and nanoparticle [13, 15] have been produced through this approach. In this study, we present a handy way to fabricate pure ZnSe nanoparticles in metastable wurtzite structure through femtosecond laser ablation technique. The structural phase transition from zinc blende to wurtzite takes place during the processing and the size of nanoparticles is controllable by adjusting the laser fluences. Additionally, the characteristics and formation mechanism of ZnSe nanoparticles was investigated.

The fs laser pulses used in this study were provided by a Ti: sapphire regenerative amplifier with 800 nm and 80 fs at a repetition rate of 5 kHz. The linearly polarized laser pulses were focused by a planoconvex fused silica cylindrical lens with the focal length of 100 mm at normal incidence. The spot size on the surface of samples is 2270 *μ*m × 54 *μ*m. The pulse energy was varied from 0 to 260 mJ/cm^{2} by using metallic neutral density filters with OD0.1–OD2 (Thorlabs ND series). A double-side polished (100) ZnSe wafer (5 mm × 5 mm × 0.5 mm) was mounted on a motorized *x*-*y*-*z* translation stage with the scanning speed of 100 *μ*m/s. After laser irradiation, a pale yellow powder, that is, ZnSe nanoparticles, was observed on the surface of a processed ZnSe crystal. Depending on the experimental purpose, the nanoparticles were preserved in two different ways, that is, dissolved in ethanol with ultrasonic waves or picked up with Scotch tape. After removing the ZnSe powder, there were many subwavelength ripples shown on the surface of a laser ablated ZnSe wafer. The direction of ripples was perpendicular to the polarization of laser beam and laser scanning path which is consistent with the scenario of the interference between incident beam and scattering laser light [16]. The morphology of ZnSe single crystals, before and after laser ablation, was examined using a scanning electron microscope (SEM). Moreover, the X-ray diffraction, the Raman scattering spectra, transmission electron microscopy (TEM), and the selected area electron diffraction were applied to identify the structure and characteristics of laser-induced ZnSe nanoparticles.

Figure 1(a) shows a typical TEM image of ZnSe nanoparticles with the smooth spherical shape. The diameters of ZnSe nanoparticles are in the range of tens nanometer. In the selected area electron diffraction (SAED) pattern, a six-fold symmetry was clearly observed in Figure 1(b). Through the analysis of distance and angles between the nearest diffraction points and the center biggest point, the crystal structure of ZnSe nanoparticles was identified as a hexagonal (wurtzite) and the orientation of each diffraction point was marked in Figure 1(b). Furthermore, the energy dispersive X-ray spectra (EDX) showed that Zn and Se are the only elements detected in the laser fabricated nanoparticles and the molar ratio of zinc and selenium is close to 1 : 1 (see the inset of Figure 1(a)). During the femtosecond laser irradiation, the dense plasma is formed on the sample surface via multiphoton absorption [17]. The ablated plume was confined near the laser focused region by surrounding air which prevents other ingredients of air, such as nitrogen, oxygen, and carbon dioxide, to get involved in the formation process of ZnSe nanoparticles under ambient environment. The size distribution of ZnSe nanoparticles fabricated at various fluences was analyzed in Figure 1(c). By fitting with the log-normal function, the average diameter of ZnSe nanoparticles was determined to be approximately 16 nm in the case of 135 mJ/cm^{2}. With an increase in the laser fluence to 198 mJ/cm^{2} and 220 mJ/cm^{2}, the average size of the ZnSe nanoparticles slightly increased to 20 nm and 22 nm, respectively. Although the variation of average size (~6 nm) is smaller than the statistic bar width of 10 nm in Figure 1(c) (determined by the variation of average size of ZnSe nanoparticles under same fluences, which is caused by the fluctuations of laser fluences, pulse durations, spectra, and so on.), the higher fluence indeed generate more ZnSe nanoparticles with larger size. This indicates that the size distribution of ZnSe nanoparticles can be controlled by adjusting laser fluence and increases as the laser fluence rises. Furthermore, the generation rate of ZnSe nanoparticles using fs laser pulses is approximately 3.63 × 10^{10} s^{−1} (or 7.26 × 10^{6} per pulse) with a fluence of 135 mJ/cm^{2}. For the higher fluence of 220 mJ/cm^{2}, the generation rate of ZnSe nanoparticles increased by one order of magnitude to 3.63 × 10^{11} s^{−1} (or 7.26 × 10^{7} per pulse).

In Figure 2(a), X-ray diffraction patterns revealed the structures of a ZnSe single-crystal wafer and the ZnSe nanoparticles fabricated under various laser fluences are zinc blende and wurtzite, respectively, according to the JCPDS card no. 80-0021 ( Å) and no. 80-0008 ( Å, Å) for ZnSe. It can be clearly seen that the zinc blende phase of a ZnSe single-crystal wafer has been transferred to the wurtzite phase in the ZnSe nanoparticles. Because wurtzite ZnSe is a metastable phase under ambient conditions, it can only be observed under high pressure and high temperature conditions. However, wurtzite ZnSe nanoparticles can be easily and reliably achieved using femtosecond laser ablation as demonstrated in this study. Additionally, the room-temperature Raman scattering spectra of samples was measured by micro-Raman system as shown in Figure 2(b). The typical Raman scattering peaks of ZnSe nanoparticles were clearly observed from 200 to 250 cm^{−1} which are rather different from that of ZnSe single crystal wafer. Moreover, there was no vibration mode due to impurities observed in the Raman spectra which is consistent with the above EDX results. A look at the Raman spectra in the case of 220 mJ/cm^{2} can be fitted well by three Lorentzian lines located at 250, 232, and 203 cm^{−1}. The peaks at 203 and 250 cm^{−1} are attributed to the transverse optical (TO) phonon mode and longitudinal optical (LO) phonon mode of ZnSe, respectively [18, 19]. Another peak located at 232 cm^{−1} between the LO and TO phonons is assigned to be the surface phonon mode () of nanoparticles. This phenomenon, appearance of surface phonon mode, can be decidedly observed in small-sized material [9, 20] due to the high surface to volume ratio and the dominant surface properties. In order to figure out the relation between TO phonon mode and surface phonon mode, the theoretical expression was used as follows [20]:
where and represent the surface phonon and TO phonon frequency, respectively; and are static and high-frequency dielectric constant, respectively; is the dielectric constant of surrounding medium and indicates the depolarization factor which is related to the particle shape. In the case of ZnSe, cm^{−1}, , , and is equal to 1 for air surrounding condition [18]. Because the laser-fabricated ZnSe nanoparticles are in spherical shape, according to the TEM image shown in Figure 1(a), the depolarization factor () is 1/3. Using (1), the calculated surface phonon mode is located at 238 cm^{−1} which is consistent with the measured value of 232 cm^{−1}. It is worth to note that the LO, TO, and surface phonon modes are strongly fluence dependent. As the laser fluence decreases, the LO and TO peaks gradually shrink; meanwhile, the surface phonon mode increases. In the case of 135 mJ/cm^{2}, the surface phonon mode almost dominates the Raman spectra, which is due to the smaller average size and more uniform size distribution as shown in Figure 1(c). Additionally, the small-size nanoparticles also result in the red shift of surface phonon mode.

According to the early researches, ZnSe transforms from a zinc blende structure to the wurtzite structure when the temperature is above the transition temperature () of 1698 K [7]. When ZnSe crystals are irradiated by the femtosecond laser pulses, the temperature of electrons and lattice in ZnSe crystals increases according to the two-temperature model [21]. Because of the much smaller heat capacity in electron subsystem, the increase of electron temperature is dramatically larger than that of lattice. The electron temperature can be described by [22]
where is the reflectivity at 800 nm and is the laser fluences and is the linear coefficient of heat capacity due to the electronic subsystem. The mean value is taken for the depth going from the crystal surface down to the skin depth *μ*m (it was estimated from the nonlinear absorption coefficient *β* [23]). In this study, taking K, (which is assumed to be totally absorbed by ZnSe), mJ/cm^{2}, and mJ mol^{−1} K^{−1} [24], we obtain K. However, for the structure transition in materials, the key factor is the lattice temperature rather than the electron temperature. Thus, we further consider the increase in the transient temperature in materials can be estimated according to the relationship of , where is the pulse energy, is the heat capacity, and is the illuminated volume. For ZnSe at 300 K, is ~1.89 ×10^{6} J/m^{3} K [7], is 2.29 × 10^{−13} m^{3} (absorption depth 1.87 *μ*m estimated from the nonlinear absorption coefficient *β* [23]), and is in the order of 0.243 mJ (which is assumed to be totally absorbed by ZnSe). Thus, the is approximately 560 K, which is far below the structural transition temperature of 1698 K. Therefore, a structural transition could not be induced by the increase in temperature. To identify the mechanism underlying the phase transition of ZnSe from zinc blende to wurtzite, we further analyzed the influence of “ablation pressure” [25], which has been studied from various perspectives over the past few decades [26, 27]. When solids are irradiated by laser pulses, high-density plasma is formed on the surface of the samples [17]. The compressed plasma in laser driven implosions has been characterized as the ablating or exploding pusher according to the surface ablation pressure and bulk pressure due to the preheating through electrons.

In 2003, Batani et al. [25] derived the shock pressure with the laser and target parameters expressed as
where is the irradiance on target with the unit of W/cm^{2}; is the laser wavelength in *μ*m; and are, respectively, the mass number and the atomic number of the target; is the time in ns. Figure 3 shows the effective pressure in the irradiated region with the laser peak power density of W/cm^{2}. In this study, the maximum pressure induced by the laser reached approximately 1.5 Mbar. According to the studies of Greene et al. in II–VI compounds [28], the solid-solid transition point, that is, the zinc blende-wurtzite phase transition, of ZnSe is approximately 0.55 Mbar. In our experiments, the ablation pressure induced by the femtosecond laser pulses on the ZnSe single crystals was in the range of 1.0 Mbar to 1.5 Mbar as shown in the shadow area of Figure 3. This exceeds the solid-solid transition pressure 0.55 Mbar (the dashed line in Figure 3). Therefore, the wurtzite-phase ZnSe nanoparticles transferred from the zinc blende phase may be caused by high ablation pressure resulting from the femtosecond laser pulses, and the accompanied increase in surface to volume ratio in the nanoparticles.

In summary, we demonstrated a simple and reliable approach to obtain the thermally metastable and pure ZnSe nanoparticles. The spherical-shape wurtzite ZnSe nanoparticles with the average diameter of <25 nm can be well produced through the femtosecond laser ablation technique. While the femtosecond laser pulses are focused on the surface of a ZnSe wafer in air, the ablated plume cannot expand as rapidly as those in vacuum chamber and then causes an instantaneous high-energy and high-pressure region around the laser focused point; meanwhile, a large amount of ZnSe nanoparticles was fabricated on the surface of a ZnSe wafer. During the formation of ZnSe nanoparticles, the structural phase further changes from the zinc blende phase to the metastable wurtzite phase due to the ultrahigh localized ablation pressure caused by the rapid injection of high laser energy within a femtosecond time scale.

#### Acknowledgments

The authors would like to express their sincere appreciation and gratitude to W. T. Chen and Professor Y. J. Hsu for their technical support. This work was supported by the MOE-ATU program at NCTU and National Science Council of Taiwan, under Grant no. NSC 98-2112-M-009-008-MY3.

#### References

- M. Bruchez, M. Moronne, P. Gin, S. Weiss, and A. P. Alivisatos, “Semiconductor nanocrystals as fluorescent biological labels,”
*Science*, vol. 281, no. 5385, pp. 2013–2016, 1998. View at Publisher · View at Google Scholar · View at Scopus - R. S. Friedman, M. C. McAlpine, D. S. Ricketts, D. Ham, and C. M. Lieber, “Nanotechnology: high-speed integrated nanowire circuits,”
*Nature*, vol. 434, no. 7037, p. 1085, 2005. View at Publisher · View at Google Scholar · View at Scopus - W. C. W. Chan and S. Nie, “Quantum dot bioconjugates for ultrasensitive nonisotopic detection,”
*Science*, vol. 281, no. 5385, pp. 2016–2018, 1998. View at Publisher · View at Google Scholar · View at Scopus - J. Che, X. Yao, H. Jian, and M. Wang, “Application and preparation of ZnSe nanometer powder by reduction process,”
*Ceramics International*, vol. 30, no. 7, pp. 1935–1938, 2004. View at Publisher · View at Google Scholar · View at Scopus - D. Sarigiannis, J. D. Peck, G. Kioseoglou, A. Petrou, and T. J. Mountziaris, “Characterization of vapor-phase-grown ZnSe nanoparticles,”
*Applied Physics Letters*, vol. 80, no. 21, pp. 4024–4026, 2002. View at Publisher · View at Google Scholar · View at Scopus - K. V. Anikin, N. N. Melnik, A. V. Simakin, G. A. Shafeev, V. V. Voronov, and A. G. Vitukhnovsky, “Formation of ZnSe and CdS quantum dots via laser ablation in liquids,”
*Chemical Physics Letters*, vol. 366, no. 3-4, pp. 357–360, 2002. View at Publisher · View at Google Scholar · View at Scopus - P. Rudolph, N. Schäfer, and T. Fukuda, “Crystal growth of ZnSe from the melt,”
*Materials Science and Engineering R*, vol. 15, no. 3, pp. 85–133, 1995. View at Google Scholar · View at Scopus - Y. P. Leung, W. C. H. Choy, I. Markov, G. K. H. Pang, H. C. Ong, and T. I. Yuk, “Synthesis of wurtzite ZnSe nanorings by thermal evaporation,”
*Applied Physics Letters*, vol. 88, no. 18, Article ID 183110, 2006. View at Publisher · View at Google Scholar · View at Scopus - C. X. Shan, Z. Liu, X. T. Zhang, C. C. Wong, and S. K. Hark, “Wurtzite ZnSe nanowires: growth, photoluminescence, and single-wire Raman properties,”
*Nanotechnology*, vol. 17, no. 22, article 006, pp. 5561–5564, 2006. View at Publisher · View at Google Scholar · View at Scopus - L. Jin, W. C. H. Choy, Y. P. Leung, T. I. Yuk, H. C. Ong, and J.-B. Wang, “Synthesis and analysis of abnormal wurtzite ZnSe nanowheels,”
*Journal of Applied Physics*, vol. 102, no. 4, Article ID 044302, 2007. View at Publisher · View at Google Scholar · View at Scopus - A. P. Joglekar, H. Liu, G. J. Spooner, E. Meyhöfer, G. Mourou, and A. J. Hunt, “A study of the deterministic character of optical damage by femtosecond laser pulses and applications to nanomachining,”
*Applied Physics B*, vol. 77, no. 1, pp. 25–30, 2003. View at Publisher · View at Google Scholar · View at Scopus - M. Y. Shen, C. H. Crouch, J. E. Carey, and E. Mazur, “Femtosecond laser-induced formation of submicrometer spikes on silicon in water,”
*Applied Physics Letters*, vol. 85, no. 23, pp. 5694–5696, 2004. View at Publisher · View at Google Scholar · View at Scopus - C. W. Luo, C. C. Lee, C. H. Li et al., “Ordered YBCO sub-micron array structures induced by pulsed femtosecond laser irradiation,”
*Optics Express*, vol. 16, no. 25, pp. 20610–20616, 2008. View at Publisher · View at Google Scholar · View at Scopus - T. Jia, M. Baba, M. Huang et al., “Femtosecond laser-induced ZnSe nanowires on the surface of a ZnSe wafer in water,”
*Solid State Communications*, vol. 141, no. 11, pp. 635–638, 2007. View at Publisher · View at Google Scholar · View at Scopus - Y. Nakata, T. Okada, and M. Maeda, “Fabrication of dot matrix, comb, and nanowire structures using laser ablation by interfered femtosecond laser beams,”
*Applied Physics Letters*, vol. 81, no. 22, pp. 4239–4241, 2002. View at Publisher · View at Google Scholar · View at Scopus - C. Wang, H.-I. Wang, W.-T. Tang, C.-W. Luo, T. Kobayashi, and J. Leu, “Superior local conductivity in self-organized nanodots on indium-tin-oxide films induced by femtosecond laser pulses,”
*Optics Express*, vol. 19, no. 24, pp. 24286–24297, 2011. View at Publisher · View at Google Scholar · View at Scopus - A. De Giacomo, M. Dell'Aglio, A. Santagata, and R. Teghil, “Early stage emission spectroscopy study of metallic titanium plasma induced in air by femtosecond- and nanosecond-laser pulses,”
*Spectrochimica Acta B*, vol. 60, no. 7-8, pp. 935–947, 2005. View at Publisher · View at Google Scholar · View at Scopus - W. Martienssen and H. Warlimont,
*Springer Handbook of Condensed Matter and Materials Data*, Springer, Berlin, Germany, 2005. - Z. D. Hu, X. F. Duan, M. Gao, Q. Chen, and L.-M. Peng, “ZnSe nanobelts and nanowires synthesized by a closed space vapor transport technique,”
*Journal of Physical Chemistry C*, vol. 111, no. 7, pp. 2987–2991, 2007. View at Publisher · View at Google Scholar · View at Scopus - S. Hayashi and H. Kanamori, “Raman scattering from the surface phonon mode in GaP microcrystals,”
*Physical Review B*, vol. 26, no. 12, pp. 7079–7082, 1982. View at Publisher · View at Google Scholar · View at Scopus - S. I. Anisimov, B. L. Kapeliovich, and T. L. Perelman, “Electron emission from metal surfaces exposed to ultrashort laser pulses,”
*Soviet Physics JETP*, vol. 39, pp. 375–377, 1974. View at Google Scholar - C. W. Luo, I. H. Wu, P. C. Cheng et al., “Quasiparticle dynamics and phonon softening in FeSe superconductors,”
*Physical Review Letters*, vol. 108, no. 25, Article ID 257006, 2012. View at Publisher · View at Google Scholar · View at Scopus - K. Y. Tseng, K. S. Wong, and G. K. L. Wong, “Femtosecond time-resolved Z-scan investigations of optical nonlinearities in ZnSe,”
*Optics Letters*, vol. 21, no. 3, pp. 180–182, 1996. View at Google Scholar · View at Scopus - J. A. Birch, “Heat capacities of ZnS, ZnSe and CdTe below 25K,”
*Journal of Physics C*, vol. 8, no. 13, Article ID 013, pp. 2043–2047, 1975. View at Publisher · View at Google Scholar · View at Scopus - D. Batani, H. Stabile, A. Ravasio et al., “Ablation pressure scaling at short laser wavelength,”
*Physical Review E*, vol. 68, no. 6, Article ID 067403, pp. 674031–674034, 2003. View at Google Scholar · View at Scopus - M. H. Key, P. T. Rumsby, R. G. Evans, C. L. S. Lewis, J. M. Ward, and R. L. Cooke, “Study of ablatively imploded spherical shells,”
*Physical Review Letters*, vol. 45, no. 22, pp. 1801–1804, 1980. View at Publisher · View at Google Scholar · View at Scopus - J. S. De Groot, K. G. Estabrook, W. L. Kruer, R. P. Drake, K. Mizuno, and S. M. Cameron, “Distributed absorption model for moderate to high laser powers,”
*Physics of Fluids B*, vol. 4, no. 3, pp. 701–707, 1992. View at Google Scholar · View at Scopus - R. G. Greene, H. Luo, and A. L. Ruoff, “High pressure X-ray and Raman study of ZnSe,”
*Journal of Physics and Chemistry of Solids*, vol. 56, no. 3-4, pp. 521–524, 1995. View at Google Scholar · View at Scopus